POUR L'OBTENTION DU GRADE DE DOCTEUR ÈS SCIENCES
acceptée sur proposition du jury: Prof. J. A. Schiffmann, président du jury Prof. R. Glardon, Dr E. Boillat, directeurs de thèse
Dr Ph. Thévoz, rapporteur Dr V. Romano, rapporteur Dr A. Jacot, rapporteur
Study and Modelling of the Melt Pool Dynamics during
Selective Laser Sintering and Melting
ÉCOLE POLYTECHNIQUE FÉDÉRALE DE LAUSANNEPRÉSENTÉE LE 26 NOVEMBRE 2015
À LA FACULTÉ DES SCIENCES ET TECHNIQUES DE L'INGÉNIEUR LABORATOIRE DE GESTION ET PROCÉDÉS DE PRODUCTION PROGRAMME DOCTORAL EN SYSTÈMES DE PRODUCTION ET ROBOTIQUE
Foremost I would like to thank my thesis directors, Rémy Glardon and Eric Boillat, for the possibility to be a part of LGPP during these four years and to work in its calm and friendly atmosphere. Thank you for your support, for the encouragement and motivation and for the patience during long discussions.
I am also grateful to the members of the thesis jury, Valerio Romano, Alain Jacot, Philippe Thévoz and Jürg Schiffmann, for the interest to my work, for the insightful comments, and for the fact, that the question session during my private defense turned into an interesting scientific discussion, which allowed me to look at my work at a new angle.
My sincere thanks to Christoph Van Gestel, Jamasp Jhabvala and Pascal Clausen for the fruitful collaboration. I am also grateful to Marc Matthey for the technical support at all time. I would particularly like to thank Ioanna Paniara and Corinne Lebet for their help in solving administrative problems.
I am very much grateful to my fellow labmates, Maryam Darvish, Christos Tsagkalidis and Nikola Kalentic for the moral support. Working with you was a pleasure.
This work would not be possible without help of my dear family. I cannot say how much I am thankful to my mother, Olga Polivnikova, for her love and support. And I will always be grateful to the members of my family, who unfortunately are no longer here, but who significantly influenced my personality: my beloved grandfather Valentin Leonov and my godfather Boris Djubua.
I would also like to thank Sergey Kolosov, a good friend of mine, for the given opportunities. And I have no words to express my gratitude to my Russian friends, Anna Popkova, Nadia Sergeeva, Yuri Sergeev, Sveta Korotkova and Ilya Koshkin, who supported me all these years, despite the distance separating us. Actually, this work I dedicate to friendship.
Selective Laser Sintering (SLS) and Selective Laser Melting (SLM) are parent layer manufac-turing processes that allow generating complex 3D parts by consolidating layers of powder material on top of each other. Consolidation is obtained by processing the selected areas using the thermal energy supplied by a focused laser beam. In SLS partial fusion of powder particles takes place, followed by a solidification of the created liquid. SLM is essentially the same pro-cess as SLS, with the difference that the particles are completely molten under the laser beam. This development is driven by the need to produce near full dense objects, with mechanical properties comparable to those of bulk materials and by the desire to avoid lengthy post processing cycles. Identification of the optimal process conditions (so-called process window) is a crucial task for industrial application of SLS/SLM processes. Operating parameters of the process are adjusted in correspondence with optical and thermal properties of the processed material. Nowadays in SLS/SLM there is a tendency to increase the speed of the fabrication as a consequence of the available higher laser powers. It leads to increase of laser scanning speeds. In these circumstances, to rely only on experimental investigations in order to adjust process and material parameters is time-consuming and ineffective. Simulation tools are strongly needed for the visualization and analysis of SLS/SLM processes.
In SLM the powder grains under the laser are completely molten and form a liquid domain called melt pool. Evolution of the melt pool during the process, its interaction with the laser, the substrate and the surrounding non-molten powder strongly affect the quality of the final part.
The goal of this work is to study the melt pool dynamics by means of a finite-element simula-tion software, built specially for SLS/SLM. The numerical model is based on the homogeneous medium hypothesis. It considers the interaction between the laser and the powder material, the phase transformations and the evolution of the material properties during the process. We also study the influence of the phase change on the process efficiency.
The macroscopic model is completed by the sub-models, which allow to study at microscopic level the processes taking place in the powder bed during its laser heating and melting. Melting of separate powder particles during laser irradiation is studied by means of the improved Single Grain Model. The capillary phenomena taking place in the powder bed during SLS/SLM are also considered. The interconnection of powder grains during their melting is approached by the mechanism of liquid drops coalescence. According to the obtained results, the depth-dependent sintering threshold for powder materials is proposed.
Key words: Selective Laser Sintering, Selective Laser Melting, powder, 18Ni(300) Maraging Steel, numerical model, finite element, temperature, enthalpy, sintering threshold, process efficiency, melt pool, stabilization, effective thermal conductivity, absorptivity, Single Grain Model, plane wave, capillary, liquid drop, coalescence.
Le frittage sélectif par laser (SLS) et la fusion sélective par laser (SLM) sont des procédés de fabrication additifs voisins qui permettent de construire des pièces 3D de géométrie compliquées en consolidant localement des couches de poudre l’une au-dessus de l’autre. Les zones à consolider sont mises en fusion grâce à l’énergie thermique fournie par un faisceau laser finement focalisé. La cohésion du matériau est obtenue après un processus de resolidification complexe. Dans le procédé SLS la fusion des particules de poudre n’est que partielle. Le procédé SLM est essentiellement le même à la différence près que les particules sont complètement fondues. Le développement du procédé SLM à partir du procédé SLS plus ancien a été motivé par la nécessité de produire des objets entièrement denses, avec des propriétés mécaniques comparables à celles des pièces obtenues en fonderie, usinage ou forgeage et sans avoir à passer par de longs cycles de post-traitement. L’identification de conditions opératoires optimales est une tâche cruciale pour l’application industrielle des procédés SLS/SLM. Dans la pratique, les paramètres du procédé sont adaptés aux propriétés optiques et thermiques du matériau utilisé. De nos jours, l’augmentation de la puissance des lasers disponibles sur le marché a permis une augmentation des vitesses de production des procédés SLS/SLM. Dans ces conditions, les approches purement expérimentales pour la mise au point des paramètres procédé sont coûteuses et relativement peu efficaces. Les outils de simulation sont donc devenus nécessaires pour l’optimisation et l’analyse des technologies SLS/SLM.
Dans le procédé SLM, les grains de poudre sous le laser sont fondus complètement. Ils forment un domaine liquide appelé bain de fusion. L’évolution de ce domaine au cours du processus, de son interaction avec le laser, le substrat et la poudre non fondue affectent fortement la qualité de la pièce finale.
Le but de ce travail est d’étudier la dynamique du bain de fusion au moyen d’un logiciel de simulation par éléments finis, adapté spécialement aux procédés SLS / SLM. Le modèle numérique est basé sur la technique mathématique d’homogénéisation du milieu traité et prend en compte de nombreux mécanismes comme l’interaction entre le laser et la poudre, les transformations de phase et l’évolution des propriétés du matériau en cours de consolidation. Nous étudions également l’influence du changement de phase sur l’efficacité du procédé. Le modèle macroscopique est complété par des sous-modèles, qui permettent d’étudier des processus qui se déroulent, à l’échelle microscopique, dans le lit de poudre lors de son traitement par laser. La fusion des particules de poudre en cours d’irradiation est étudiée au moyen d’une généralisation du modèle classique du grain isolé. Les phénomènes de capillarité
se produisant dans le lit de poudre pendant les procédés SLS/SLM sont également étudiés. En particulier, l’interconnection des grains de poudre en cours de fusion est analysée grâce à des modèles (théoriques et numériques) de coalescence de gouttes. Les résultats obtenus ont notamment conduit à la définition d’un seuil de frittage dépendant de l’intensité du faisceau laser et de ses propriétés de pénétration dans la poudre.
Mots clefs : frittage sélectif par laser, fusion sélective par laser, poudre, acier maraging 18Ni (300), modèle numérique, éléments finis, température, enthalpie, seuil de frittage, efficacité des processus, bain de fusion, stabilisation, conductivité thermique effective, absorption effec-tive, modèle du grain isolé, onde plane, écoulement capillaire, goutte de liquide, coalescence.
Abstract (English/Français) iii
List of figures xi
List of tables xiii
. . . xv
List of symbols xv 1 Introduction 1 1.1 Research objectives . . . 3
1.2 Thesis structure . . . 4
2 State of the Art 5 2.1 SLS/SLM process definition . . . 6
2.1.1 Binding mechanisms . . . 7
2.1.2 Materials and applications . . . 7
2.1.3 Requirements to the process . . . 8
2.2 Characterization of SLS/SLM process . . . 9
2.2.1 Process parameters . . . 9
2.2.2 Material parameters . . . 10
2.3 Numerical modelling of SLS/SLM . . . 10
3 18Ni(300) Maraging Steel Powder 13 3.1 Grain size distribution . . . 14
3.2 Bulk material properties . . . 15
3.3 Powder properties . . . 16
3.3.1 Surface absorptivity and optical penetration depth . . . 16
3.3.2 Powder density . . . 20
3.3.3 Effective thermal conductivity . . . 20
3.4 Molten material properties . . . 22
3.5 Operation parameters used for Maraging Steel Powder . . . 23
4 Single Grain Model 25
4.1 Single Grain Model: main assumptions . . . 26
4.1.1 Intensity of the plane wave and laser power . . . 27
4.1.2 Heating of a spherical grain with a plane wave . . . 28
4.2 Melting of a powder grain . . . 29
4.3 Evolution of powder bed properties . . . 31
4.4 Different powder grain sizes . . . 35
4.5 Conclusions . . . 37
5 Melting Dynamics 39 5.1 Capillary properties of molten powder material . . . 40
5.1.1 Dynamic viscosity . . . 40
5.1.2 Surface tension . . . 41
5.1.3 Summary . . . 42
5.2 Liquid drops coalescence model . . . 43
5.3 Conclusions . . . 49
6 Numerical Modelling of SLS/SLM 51 6.1 Numerical model description . . . 52
6.1.1 Enthalpy and temperature evolution . . . 52
6.1.2 Sintering potential and effective properties . . . 53
6.1.3 Sintering potential evolution . . . 54
6.2 Numerical method . . . 55
6.2.1 Time discretization . . . 55
6.2.2 Space discretization . . . 57
7 Sintering Threshold in SLS/SLM 61 7.1 Evolution of the grain melting threshold . . . 62
7.2 Process parameters and material properties . . . 65
7.3 Simulation results . . . 66
7.4 Conclusions . . . 68
8 Mechanisms Affecting the Efficiency of SLS/SLM Process 69 8.1 Thermal conductivity and absorptivity evolution in SLS/SLM . . . 70
8.1.1 Simulation: constant material properties . . . 70
8.1.2 Rosenthal solution . . . 71
8.1.3 Simulation: evolving material properties . . . 73
8.1.4 Influence of absorptivity evolution on SLS/SLM efficiency . . . 74
8.2 Convection and radiation . . . 76
8.2.1 Convection . . . 77
8.2.2 Radiation . . . 80
8.3 Conclusions . . . 81 viii
9 Melt Pool Dynamics 83
9.1 Bulk material . . . 84
9.2 Powder bed . . . 86
9.3 Powder layer on a substrate . . . 87
9.4 Theoretical model . . . 88
9.5 Stabilization distance . . . 92
9.6 Different scanning strategies . . . 93
9.7 Conclusions . . . 96
10 Conclusions 97
List of Figures
2.1 The SLS process scheme . . . 6
3.1 18Ni(300) Maraging Steel Powder. . . 14
3.2 Grain size distribution of the 18Ni(300) Maraging Steel powder . . . 14
3.3 β-function for 18Ni(300) Maraging Steel. . . 17
3.4 Radiation reflection, transmission and absorption. . . 18
3.5 Discrete thermal resistances model for powder beds by A.V. Gusarov (pic. ). . 20
4.1 Irradiation of the surface of a powder bed by a moving laser. . . 26
4.2 Meshing of a 2D domain for the Single Grain Model calculations. . . 28
4.3 Temperature distribution inside a spherical grain after 6µs of irradiation by the plane wave with the intensity corresponding to the 100 W laser (Tab. 4.1). . . . 29
4.4 Evolution of molten material proportion during grain melting by a plane wave of different intensities approaching laser beam with power 100 W, 200 W, 300 W. 30 4.5 Maximum irradiation of a powder grain by a top-hat laser beam. . . 31
4.6 Evolution of the proportion of the molten material during irradiation of two neighbouring grains: (i) t < t0; (ii) t ' t0, (iii) t > t0. . . 32
4.7 Temperature evolution in the contact point between two grains irradiated by a plane wave, approaching the laser of different powers. . . 33
4.8 Evolution of the average temperature of a powder grain (Tab. 4.1), irradiated by a plane wave, approaching the laser of different powers. . . 34
4.9 Single Grain Model: Time to the contact spot melting t0and average temperature Tav0 of the powder grain at the moment t0. . . 36
5.1 The dynamic viscosity of pure liquid iron in the range of temperatures 1538◦C < T < 2500◦C . . . 40
5.2 Coalescence of two liquid drops. . . 43
5.3 Relative contact spot radius evolution: simulation and theoretical results, r0= 4.435µm . . . 45
5.4 Relative contact spot radius evolution for different radii of liquid drops: solid lines – LFEM, dashed lines – Shikhmurzaev’s eq. (5.9) and Thorrodsen’s eq. (5.7). 46 5.5 Contact spot radius evolution between two liquid drops of different radii: (i) r1= 2.5 µm, r2= 4.435 µm; (ii) r1= 4.435 µm, r2= 10 µm (eq. (5.11)). . . . 47
List of Figures
6.1 Typical domainΩ: powder bed (with top surface Σ) on a substrate. . . 52 6.2 Illustration of the net of parallelepipedic cells for the space discretization of the
sintering potentialΦ. . . 57 6.3 Top view of the non conformal mesh for the temperature/enthalpy profiles. . . 60 7.1 Evolution of the molten material fraction and the average temperature of a
18Ni(300) Maraging Steel powder grain for different laser powers. . . 62 7.2 The dependency of the grain melting threshold TtSGMon the wave intensity. . . 63 7.3 The dependency of the melting threshold on the depth for wave intensities,
approaching laser powers 100 W, 200 W, 300 W. . . 64 7.4 Exact laser path and explanation of the laser delay. . . 65 7.5 Time above the sintering threshold when Tt = TtSGM (solid lines) and when
Tt= Tf (dashed lines) for Sets I and II (Tab. 7.2). . . 67 7.6 EBSD analysis of the results for sets I and II (Tab. 7.2). Provided by Dr. J.Jhabvala. 68 8.1 Influence of the thermal conductivity and absorptivity evolution on the
maxi-mum temperature reached on the surface of the material during laser scanning (see Tab. 8.1). . . 73 8.2 Absorption of laser power in the beginning of the scanning for 18Ni(300)
Marag-ing Steel powder. . . 74 8.3 Approximate position of the stabilized melt pool with respect to the laser spot:
P = 300 W, υ = 1 m/s, ω = 40 µm (by Mathematica software). . . . 78 9.1 Evolution of the melt pool surface area during laser scanning of 18Ni(300)
Marag-ing Steel powder and bulk material (Tab. 3.6). . . 85 9.2 Melt pool evolution during melting of 32µm powder layer on a substrate: P = 100
W,υ = 1 m/s. . . 87 9.3 Temperature evolution according to (9.1): 0.1, 0.3, 0.5, 0.7, 0.9 ms (from the right
to the left) from the laser irradiation start: P = 100 W, υ = 1 m/s. . . . 89 9.4 Scanning strategy used for the numerical modelling in § 9.6. . . 93 9.5 Melt pool evolution during scanning of the strategy Fig. 9.4: P = 100 W, υ = 1 m/s. 94 9.6 Overlapping of scanned tracks for the strategy Fig. 9.4 and top-hat laser beam of
radius 40µm. . . 95
List of Tables
3.1 18Ni(300) Maraging Steel chemical composition . . . 15
3.2 18Ni(300) Maraging Steel bulk material properties. . . 15
3.3 Thermal conductivity of powders in air at normal conditions: theoretical predic-tion and experimental results. . . 21
3.4 Process parameters used in the study. . . 23
3.5 Sets of the process parameters used in simulation. . . 23
3.6 Properties of 18Ni(300) Maraging Steel. . . 24
4.1 Properties of the laser and of a typical 18Ni(300) Maraging Steel powder grain. . 27
4.2 Single Grain Model. (i) ts: start of the grain melting (Tab. 4.1); (ii) tl: complete grain melting; (iii) tmaxi : maximum time of grain irradiation (Fig. 4.5). . . 30
4.3 Melting time t0of the contact point between two grains, irradiated by a plane wave of intensity I0, and the average temperature Tav0 of the grains at this moment. 33 5.1 Properties of liquid 18Ni(300) Maraging Steel, used in Chapter 5. . . 42
5.2 Parameter K2(see eq.(5.7)) for different temperatures and radii of the drops . 44 5.3 Coalescence time of equal liquid drops. . . 46
5.4 Coalescence time of liquid drops with different radii. . . 48
7.1 Melting threshold TtSGMof a 18Ni(300) Maraging Steel powder grain, irradiated by a plane wave of intensity I0, approaching the laser of power P . . . . 62
7.2 Sets of process parameters. . . 66
8.1 Influence of the thermal conductivity and absorptivity evolution on the maxi-mum temperature reached under the laser: simulation vs. Rosenthal solution (8.4). . . 70
8.2 Stabilization time of the surface state within the laser spot. . . 75
9.1 Time to stabilize the melt pool for different process and material parameters. . 84
9.2 Melt pool depth reached during laser melting of 18Ni(300) Maraging Steel powder. 86 9.3 Material properties used for the estimation of the melt pool stabilization time. 91 9.4 Melt pool stabilization distance for different process and material parameters. 92 9.5 Simulation parameters for the scanning strategy presented in Fig. 9.4. . . 93
List of Symbols
Amp Surface area of the stabilized melt pool
Cp Heat capacity
Esurfd Surface laser energy density
Evold Volume laser energy density
Ea Activation energy
I0 Incident radiation intensity
Ir Reflected radiation intensity
Lc Characteristic length
Lf Latent heat of fusion
Lv Latent heat of vaporization
Mth Powder grain thermal mass
N Mean coordination number P Laser power
Q Intensity distribution of the heat source R Reflectivity of the material
Rg Universal gas constant
T0 Temperature of the environment
Tav0 Average temperature of the grain at the moment t0(SGM)
Tt Melting threshold temperature
TtSGM Melting threashold of the powder grain
Tv Boiling temperature Ω Working domain Φ Sintering potential
Σp Contact thermal resistance between two powder particles α Surface absorptivity of the material
αl Surface absorptivity of liquid material αp Surface absorptivity of the powder αs Surface absorptivity of solid material δ Optical penetration depth of the material
δ0 Radius of the sphere, used for temperature averaging η Thermal diffusivity
γ Liquid-gas surface tension
γa Adiabatic exponent of the gas phase κ Thermal exchange coefficient
E0 Electric amplitude of the plane wave
st Poynting vector
Bo Bond number Kn Knudsen number Nul Nusselt number Ral Rayleigh number
µ Dynamic viscosity of the liquid µp Vacuum magnetic permeability ω Laser beam radius
ρl Liquid material density xvi
ρp Powder density ρs Solid material density σ Stefan-Boltzmann constant
τM Maxwell relaxation time of the liquid
τsint Characteristic sintering time of the material υ Laser scanning speed
ε Material emissivity
εI Imaginary part of the dielectric constant εR Real part of the dielectric constant εd Dielectric constant
ζ Sintering rate
d0 Powder grain diameter
dmpb Melt pool stabilization distance for the bulk material
dmppl Melt pool stabilization distance for the powder layer
dmpth Theoretical stabilization distance of the melt pool
fs Fraction of the solid material
g Gravitational acceleration
hpbmp Melt pool depth in the powder bed
hh Hatching distance
hl Powder layer thickness
k Effective thermal conductivity
katm Thermal conductivity of the surrounding atmosphere
kg Thermal conductivity of gas phase
kl Effective thermal conductivity of liquid material
ks Effective thermal conductivity of solid material
l0 Gas mean-free path
qabs Heat flux corresponding to absorbed heat
qconv Heat flux corresponding to convective heat losses
qrad Heat flux corresponding to radiative heat losses
qsurf Surface heat source
r0 Powder grain radius
rc Contact radius
t0 Time of contact point melting (SGM)
ttr Transition time of the surface state within the laser spot
tmaxi Maximum time of the grain irradiation (SGM)
tl Time of complete grain melting (SGM)
ts Time to melting of the powder grain (SGM)
tatt Time when the melt pool touches the substrate
tmpb Melt pool stabilization time for bulk material
tmppb Melt pool stabilization time for powder bed
tmppl Melt pool stabilization time for powder layer on the substrate
tmpth Theoretical melt pool stabilization time
tc Time of liquid drops coalescence
u Enthalpy per unit mass
Selective Laser Sintering (SLS) and Selective Laser Melting (SLM) are parent layer manufac-turing processes that allow generating complex 3D parts by consolidating layers of metallic, ceramic, or polymer powder material on top of each other. Consolidation is obtained by processing the selected areas using the thermal energy supplied by a focused laser beam. In SLS partial fusion of powder particles takes place, followed by a solidification of the created liquid. SLM is essentially the same process as SLS, with the difference that the particles are completely molten under the laser beam and form a liquid domain called melt pool. The main advantages of SLS/SLM are three-dimensional geometrical freedom, complying with modern design requirements, mass customization and material flexibility.
Industrial application of SLS/SLM technologies requires from the process rather strict condi-tions to be fulfilled: porosity, hardness, surface roughness, geometrical accuracy and other properties of the final part should be sufficient to guarantee its reliability over the entire life cycle. The economical aspects – production time and cost – also should be considered. SLS/SLM operating parameters (so-called process window) are adjusted in correspondence with optical and thermal properties of the material. Nowadays in SLS/SLM there is a tendency to increase the speed of the fabrication as a consequence of the available higher laser powers. Identification of the optimal process parameters is a crucial task for industrial application of SLS/SLM.
Efficiency of SLM process and the quality of the final part are strongly connected to the evolution of the melt pool during the process, its interaction with the laser, the substrate and the surrounding non-molten powder. Knowledge of the melt pool geometry allows to adjust such important operating parameters as hatching distance of the scanning strategy and powder layer thickness. Prediction of the melt pool surface area evolution and melt pool position with respect to the laser helps to estimate and increase process efficiency and can be also useful for the calibration of online monitoring systems for Selective Laser Melting.
Chapter 1. Introduction
Parameters of the melt pool and the character of its interaction with the laser radiation during SLM are defined by the evolution of thermal and optical properties of the powder due to its melting. Physical laws, describing this evolution, are related to the phenomena taking place in the powder at the level of powder grains: to their melting dynamics and their interaction in the presence of the liquid phase.
We can see that SLS/SLM processes involve dynamical phenomena, strongly dependent on numerous parameters. To rely only on experimental investigations in this case is time-consuming, ineffective and expensive. Numerical modelling of SLS/SLM is strongly needed. All numerical approaches, developed for SLS/SLM, describe a working domain (a powder on a substrate) with some thermal and mechanical properties and certain boundary conditions and a heat source of a specified profile shape, which interacts with the domain. One of the commonly used modelling methods is based on the description of the heat transfer in the homogenized working domain, characterized by its effective properties. However, as mentioned above, it is clear that for better understanding of SLS/SLM it is necessary to consider the process at microscopic level, i.e. at the level of powder grains. Generally it leads to the increase of numerical model complexity and, consequently, to the decrease of computation speeds.
The solution to this problem is in the use of a numerical model based on material homoge-nization, completed with separate sub-models simulating the process at the powder grain level. The sub-models can be divided in two categories:
• models, describing the effective properties of a loose powder;
• models, studying powder grain melting dynamics and their interaction in the presence of the liquid phase.
Results of these sub-models, added to the basic macroscopic model, will allow to simulate the SLS/SLM even in the absence of large computing powers.
1.1. Research objectives
1.1 Research objectives
This study will focus on the following objectives:
1. Development of theoretical models for the description of the loose powder effective prop-erties.
2. Development of theoretical models describing the melting dynamics and the interactions of molten powder particles during SLS/SLM.
3. Theoretical investigation and numerical simulation of SLS/SLM using a macroscopic model based on the homogeneous medium hypothesis, completed by the results of micro-scopic sub-models.
4. Estimation of the influence of material properties evolution on SLS/SLM process efficiency. 5. Study of the properties and dynamics of the melt pool formed during SLM process.
This work is mainly concerned by the study of SLS and SLM of 18Ni(300) Maraging Steel pow-der. The considered operating parameters are chosen in accordance with modern industrial requirements.
Chapter 1. Introduction
1.2 Thesis structure
The structure of this work is as follows. Chapter 2 introduces main principles of Selective Laser Sintering and Selective Laser Melting. It also discusses process requirements and describes commonly used approaches for the numerical simulation of SLS/SLM.
In Chapter 3, 18Ni(300) Maraging Steel is studied. Properties of the solid and liquid phases of the material are discussed. Different methods for estimating the effective powder parameters are also introduced. The process parameters, chosen in the context of this study, are also presented.
In Chapters 4 and 5, we introduce the models studying SLS/SLM at the powder grain level. In Chapter 4, using the improved Single Grain Model, we study melting of a separate powder particle. We approach laser irradiation by a plane wave. Melting time and threshold tempera-ture of a powder grain are estimated. Chapter 5 focuses on the capillary phenomena taking place in the powder during melting. The dynamics of molten powder grain interconnection is considered in the framework of the liquid drop coalescence model.
Chapter 6 describes the numerical methods used to discretize the macroscopic SLS/SLM model. Theoretical assumptions, based on the results of Chapters 4 and 5, are presented. Recommendations about the space and time discretization are given.
Chapter 7 introduces a model for a depth-dependent sintering threshold, based on the results of the Single Grain Model (Chapter 4). An experimental validation of this model is also presented.
Chapter 8 focuses on phenomena, taking place during SLS/SLM, which can influence the process efficiency. The evolution of powder effective parameters due to the phase change is studied, convective and radiative losses are estimated.
In Chapter 9 the melt pool dynamics during SLM is discussed. Evolution of the melt pool during the process is studied and melt pool stabilization criteria are presented. A method to adjust the powder layer thickness, according to material and process parameters, is also introduced.
State of the Art
Selective Laser Sintering (SLS) and Selective Laser Melting (SLM) are parent Additive Manufac-turing processes using a laser to melt and solidify metallic, ceramic, polymer or composite powders. Additive manufacturing is the name given to a host of related technologies used to create physical objects by sequential deposition of material layers. The originality of Additive Manufacturing is that material is added to form the desired part and not subtracted from a bigger part. All the non-used material can be recycled in the next construction.
Chapter 2. State of the Art
Figure 2.1 – The SLS process scheme .
2.1 SLS/SLM process definition
Selective Laser Sintering (SLS) is a layer manufacturing process that allows generating complex 3D parts by consolidating layers of powder material on top of each other [6, 7]. The object is built layer by layer. Consolidation is obtained by processing the selected areas using the thermal energy supplied by a focused laser beam (Fig. 2.1). Using a beam deflection system, each layer is scanned according to its corresponding cross-section as calculated from the CAD model. Partial fusion of the particles takes place, followed by a solidification of the created liquid.
Selective Laser Melting (SLM) is essentially the same process as SLS, with the difference that the particles are completely molten under the laser beam and form a liquid bath (a melt pool). This development was driven by the need to produce near full dense objects, with mechanical properties comparable to those of bulk materials and by the desire to avoid lengthy post-processing cycles.
The main advantages of SLS/SLM are three-dimensional geometrical freedom, complying with modern design requirements, mass customization and material flexibility. In contrast to material removal techniques, complex parts can be fabricated without the need for lengthy tool path calculations. Shapes that may not be realizable by conventional machining can be built (conformal cooling channels in injection molds) . SLS/SLM technology makes it possible to create fully functional parts directly from metals, ceramics and plastics without using any intermediate binders or any additional processing steps after the laser sintering operation [8, 9, 10, 11]. Remaining unprocessed powder can be reused.
2.1. SLS/SLM process definition
2.1.1 Binding mechanisms
Different binding mechanisms can be responsible for the consolidation of the powder during SLS and SLM processes [12, 13, 14]:
• Solid State Sintering (SSS). Occurs below the material melting temperature: diffusion of atoms in solid state (volume diffusion, grain boundary diffusion or surface diffusion [15, 16]) creates necks between adjacent powder particles growing with time [17, 18]. The mechanism is rarely applied as diffusion of atoms in solid state is slow and does not meet the requirements of the process.
• Liquid Phase Sintering (LPS). Part of the powder material is molten while other parts remain solid. The liquefied material spreads between the solid particles almost instan-taneously as it is driven by intense capillary forces. The material that melts may be different from the one remaining solid: the ‘low melting point’ material is called the binder, while the ‘high melting point’ material is generally called the structural material. The binder may remain as part of the final product or may be removed during a debind-ing cycle. Binder and structural materials can be brought together simply by usdebind-ing a mixture of two-component powders, or they can be combined in composite or coated powders.
• Partial Melting. The heat supplied to a powder particle is sufficient only to melt the grain surface, while particle core remains solid. The molten material plays the role of the binder. Small necks are formed between the non-molten particle cores . This binding mechanism is used for metals. The technique is sometimes called Direct Metal
Laser Sintering (DMLS) .
• Full Melting. Applied to achieve fully dense parts without need for any post-processing. One of the most popular technologies nowadays. However, to achieve satisfactory results, requires a detailed preliminary analysis of the material and process parameters (so-called process window). For each new material, a process-window needs to be determined separately, in order to avoid scan track instabilities (sphereodisation of the liquid melt pool, also known as ‘balling’) and part porosity [19, 20].
2.1.2 Materials and applications
SLS/SLM technologies are widely used in various industries, medicine and research, offering a range of advantages compared to conventional manufacturing techniques. Most of the materials, used in SLS/SLM, are developed by machine makers and are strictly application-oriented [14, 21].
Chapter 2. State of the Art
• Metals. Iron-based powders and various steels (moulds and tools [22, 23, 24]), titanium-based powders and Co-Cr (implants and scaffolds).
• Polymers. Polyamide, polystyrene and PEEK (SLS plastics), PCL (biomedical applica-tions), PVA, PC.
• Ceramics. HA, SiC, ZrO2, Al2O3, glass-ceramic, Ta2O5, bismuth titanate. Least-processed materials by SLS/SLM, as far as they are susceptible to develop cracks.
2.1.3 Requirements to the process
Industrial application of Selective Laser Sintering/Melting requires from the process rather strict conditions to be fulfilled: porosity, hardness, surface roughness, geometrical accuracy and other properties should be sufficient to guarantee the reliability of the final product over the entire life cycle. It is also necessary to consider the economical aspects of the process – production time and cost.
Laser power and laser scanning speed are adjusted in correspondence with optical and thermal properties of the process material. In the case of polymers and composites the technique is now well understood and widely used, but for metals and ceramics it still suffers from a lack of precision, surface roughness and poor mechanical properties. Identification of the optimal process parameters (process window) is a crucial task for industrial application of SLS/SLM processes.
According to the industrial requirements, nowadays in SLS/SLM there is a tendency to increase the speed of the fabrication as a consequence of the available higher laser powers (up to 1 kW). For metal powders it leads to increase of scanning speeds (up to 3 − 4 m/s).
2.2. Characterization of SLS/SLM process
2.2 Characterization of SLS/SLM process
Material and process parameters, listed in §§ 2.1.2 – 2.1.3, are strongly related to each other. Laser and scanning parameters are adjusted according to chemical, optical and heat transfer properties of the processed material.
2.2.1 Process parameters
The relation between laser and strategy parameters defines the amount of energy received by a processed material and, subsequently, is of a great influence on the product properties. It would be convenient to have a variable which can link all the process parameters and, therefore characterize SLS/SLM process.
Laser energy density is a commonly used factor to characterize SLS/SLM process and proper-ties of a final sintered part. Generally energy density can connect laser power, scanning speed, hatching distance of the scanning strategy, laser beam diameter and thickness of the powder layer.
According to [25, 26, 27, 28] surface laser energy density Esurfd (in J/m2) can be expressed as:
Esurfd = P υhh
, or Esurfd = P
where P is the laser power,υ – the scanning speed, hh – the hatching distance andω – the radius of the laser beam.
An expansion of the expression (2.1) is proposed in : Esurfd = P
where ratio x = 2ω/hhcharacterizes the overlapping of the trace of a laser beam spot.
Volume based laser energy density Evold (in J/m3) is also widely used for the characterization of SLS/SLM processes :
Evold = P υhhhl
where hlis the thickness of a powder layer.
However, it can be seen, that volumic density of laser energy doesn’t take into account the diameter of the laser beam and the beam profile. Therefore, it can be reasonable to add another factor, characterizing the laser – laser intensity or laser fluence.
Chapter 2. State of the Art
In fact, no one of the parameters (2.1) – (2.3) reflects all the details of the Selective Laser Sintering/Melting process due to its non-linearities. We will discuss this problem in detail in the next chapters.
2.2.2 Material parameters
One of the commonly used methods to characterize a powder is to consider it as a homo-geneous medium with some effective properties. We will discuss this model in detail in Chapter 6.
In the framework of the homogeneous medium hypothesis, a powder bed, like any homoge-neous material, can be characterized by its thermal diffusivityη= k/ρ/Cp, where Cpis the heat capacity of the material,ρ is the powder bed density and k is the effective value of its thermal conductivity. Optical parameters of a powder bed are described by its effective surface absorptivity and optical penetration depth.
During SLS/SLM powder properties evolve to the parameters of a bulk material. In this study we will discuss the consequences of this evolution.
However it is clear, that the modification of parameters during laser sintering/melting is the result of changes in the structure of the powder bed. For better understanding of SLS/SLM at macroscopic level, we need to consider processes, which take place at the level of a powder particle, like melting, rearrangement and interaction of powder grains. Therefore powder properties (packing, grain size distribution, etc.) strongly influence the process.
2.3 Numerical modelling of SLS/SLM
The complexity of SLS/SLM processes is that they involve dynamical phenomena, caused by a time dependent temperature distribution . These phenomena are strongly dependent on many parameters. Process variables for SLS/SLM technologies can be divided in several groups:
(a) Material properties: Chemical composition, size distribution, shape, optical and heat transfer properties of powder and molten material.
(b) Laser parameters: Laser power, spot size, beam spatial distribution, scanning speed, possibly pulse rate and duration.
(c) Strategy of manufacturing: Scanning strategy, powder deposition parameters, powder layer thickness, application of a protective atmosphere, preheating.
To rely only on experimental investigations in order to adjust process and material parameters is time-consuming, ineffective and expensive. Simulation tools are strongly needed for the visualization and analysis of SLS/SLM processes.
2.3. Numerical modelling of SLS/SLM
All numerical approaches, developed for SLS/SLM modelling, describe a powder bed with some thermo-mechanical properties and certain boundary conditions and a heat source of a specified profile shape, which interacts with the powder bed. First attempts aiming to describe theoretically the mechanisms of the heat transfer in a powder bed were made in [17, 32, 33]. Mathematical models of the heat distribution for single scan tracks were proposed in [34, 35]. In  an analytical model was used to evaluate the temperature field created in a titanium sample during pulsed laser treatment. Finite element analysis by means of commercial software was performed in  for laser enamelling. A finite element numerical model, based on the relations between specific enthalpy, temperature and sintering potential, was introduced in  (see Chapter 6 for details). In  the transient temperature field for TiAl6V4SLM parts was predicted. A 3D model for the analysis of the relations between the process parameters and the mass of a powder layer was proposed in .
All these models, described above, are based on the homogenization of a powder bed. However the question of interaction of laser radiation with a powder, considered as a packing of particles, was also studied. Numerical model, based on the solution of Radiation Transfer Equation (RTE) for the absorbing and scattering medium was proposed in [41, 42]. For the same purpose ray-tracing modeling was used in [7, 43].
Evolution of effective thermal parameters of a powder bed during SLS/SLM was studied in [38, 44, 45, 46].
Nowadays there is a tendency to model SLS/SLM processes not only at macroscopic, but also at microscopic level, aiming to study powder melting dynamics. These models are often based on the solution of Navier-Stokes equations (for example ). However the lattice Boltzmann method (LBM) becomes more popular .
18Ni(300) Maraging Steel Powder
This work is mainly concerned by the study of Selective Laser Sintering and Selective Laser Melting of 18Ni(300) Maraging Steel powder. In this Chapter we describe the properties of the bulk material. We also discuss the effective values of the thermal conductivity and of the light absorptivity in the loose powder. We introduce different methods to estimate the effective parameters. For the estimation of the effective powder absorptivity we use a theoretical approach based on the solution of the radiation transfer equation. For the calculation of the effective thermal conductivity of a powder bed we apply a discrete thermal resistances model. We also introduce an experimental validation of these theoretical methods.
Chapter 3. 18Ni(300) Maraging Steel Powder
Figure 3.1 – 18Ni(300) Maraging Steel Powder.
3.1 Grain size distribution
The photo of 18Ni(300) Maraging Steel powder we study is shown in Fig. 3.1. The grain size distribution of the powder can be seen in Fig. 3.2 . In this work the details of the real distri-bution will not really be taken into account. Instead we will often approach it by a monosized distribution for a diameter d0= 8.87 µm, which corresponds to a radius r0= 4.435 µm.
Grain size,µm % number of g ra in s 0.0 5.0 10.0 15.0 20.0 25.0 30.0 35.0 40.0 45.0 50.0 0.0 2.0 4.0 6.0 8.0 10.0 12.0 14.0 16.0 18.0 20.0 d0
Figure 3.2 – Grain size distribution of the 18Ni(300) Maraging Steel powder .
3.2. Bulk material properties Aluminum, Al 0.10 % Boron, B ≤ 0.0030 % Carbon, C ≤ 0.030 % Cobalt, Co 9.0 % Iron, Fe 67.0 % Manganese, Mn ≤ 0.10 % Molybdenum, Mo 4.80 % Nickel, Ni 18.5 % Phosphorous, P ≤ 0.010 % Silicon, Si ≤ 0.10 % Sulfur, S ≤ 0.010 % Titanium, Ti 0.60 % Zirconium, Zr 0.010 %
Table 3.1 – 18Ni(300) Maraging Steel chemical composition . Density of the solid materialρs 0.008 g/mm3
Thermal conductivity ks 26 W/m/◦C
Heat capacity Cp(for T > 1091◦C) 0.5 J/g/◦C
Melting temperature Tf 1413◦C
Boiling temperature Tv 2862◦C
Latent heat of fusion Lf 247 J/g
Latent heat of vaporization Lv 6260 J/g
Table 3.2 – 18Ni(300) Maraging Steel bulk material properties.
3.2 Bulk material properties
The chemical composition of the 18Ni(300) Maraging Steel bulk material is given in Tab. 3.1. Other physical properties are presented in Tab. 3.2. According to , we assume Tf = 1413◦C as the material melting point. Due to lack of complete information, they do not all correspond exactly to 18Ni(300) Maraging Steel. Sometimes they have been interpolated from the proper-ties of pure iron or close grades of steel. The values Lf and Lvcorrespond to the latent heat of fusion and latent heat of vaporization of Grade 316 Stainless Steel, respectively [49, 50]. For Tv we take the vaporization point of iron.
According to , the densityρsof 18Ni(300) Maraging Steel is not dependent on temperature. The thermal conductivity of the material at 50◦C is ks= 25.8 W/m/◦C . We round this value to 26 W/m/◦C and assume it to be constant. The heat capacity Cp strongly depends on temperature. The value given in Tab. 3.2 (Cp= 0.5 J/g/◦C) will only be used for tempera-tures T > 1091◦C. For smaller values of T , the heat capacity can be deduced from the data concerning theβ-function of the material (see Fig. 3.3).
Chapter 3. 18Ni(300) Maraging Steel Powder
In Chapter 6, describing the numerical model, we will use the so-calledβ-function, which connects the enthalpy per unit mass u to the temperature T . Theβ-function of 18Ni(300) Maraging Steel has been measured by EMPA  for u < 598.9 J/g and under the assumption thatβ(0) = 0 which means that
u = 0 J/g, when T = 0◦C. (3.1)
For values of u larger than 598.9 J/g, theβ-function is constructed under the assumption that Cp' 0.5 J/g/◦C and by taking the values of Lf, Lv, Tf and Tvinto account (see Tab. 3.2). The final result is presented in Fig. 3.3. Fig. 3.3b is the zooming of the grey area on the graph Fig. 3.3a.
3.3 Powder properties
As it will be explained in detail in Chapter 6, we will consider the powder bed as a homoge-neous medium, which is characterized by effective properties: surface absorptivity, optical penetration depth, thermal conductivity and density. These parameters strongly depend on powder geometry and material properties.
In this section we present methods to estimate the effective properties. We also discuss assumptions we have to make for the 18Ni(300) Maraging Steel powder.
3.3.1 Surface absorptivity and optical penetration depth
The ability of a powder to absorb laser energy is one of the key factors for the SLS/SLM process quality. In general, when electromagnetic radiation is incident to the surface of a medium, it is partially reflected from the surface and partially penetrates into the material (Fig. 3.4). The reflected part of the radiation Ir, if non-linear phenomena are neglected, can be expressed as:
Ir= R I0, (3.2)
where I0is the intensity of the incident radiation and R is the reflectivity (or the reflection coefficient) of the material. Further in this study, to characterize the ability of the material to absorb radiation, we will use the notion of the surface absorptivity:
α = 1 − R. (3.3)
In fact, surface absorptivity of a medium is defined as the fraction of the incident radiation which penetrates into the medium.
3.3. Powder properties Enthalpy u, J/g T emp er at u re T , ◦ C 0.0 1000 2000 3000 4000 5000 6000 7000 8000 9000 0.0 700 1400 2100 2800 3500 4200
Tv transition liquid → gas
gas phase li quid p h ase Lv
(a)β-function for 18Ni(300) Maraging Steel.
Enthalpy u, J/g T emp er at u re T , ◦ C 0.0 100 200 300 400 500 600 700 800 900 1000 1100 1200 1300 0.0 200 400 600 800 1000 1200 1400 1600 1800 2000 trans. solid → liq. Tf li quid p h ase sol id phase Lf
(b)β-function for 18Ni(300) Maraging Steel (zoom of the grey region).
Chapter 3. 18Ni(300) Maraging Steel Powder
Figure 3.4 – Radiation reflection, transmission and absorption.
During propagation in the medium, the non-reflected radiation is partially absorbed by the material. In the case of a plane electromagnetic wave, propagating in a homogeneous medium along direction z, perpendicular to the medium surface, the radiation intensity decay according to Beer-Lambert law. The intensity of the transmitted radiation at a distance z from the material layer surface (see Fig. 3.4) is:
Itr(z) = αI0e−z/δ, (3.4)
whereδ is the optical penetration depth of the material, I0– the incident intensity andα – the surface absorptivity (see (3.2)–(3.3))
If the incident radiation is not a plane wave but a Gaussian beam (TEM00) the law (3.4) generalizes under some conditions . These conditions are:
(i) the material surface corresponds the waist plane of the beam; (ii) the distance z is relatively small compared to the beam radiusω:
z ¿ kλω2, (3.5)
where kλ= 2π/λ is the wave number, λ – the laser wavelength.
In such a situation, one may write:
Itr(x, y, z) ' αI0(x, y)e−z/δ (3.6)
with I0(x, y), the incident gaussian beam intensity at location (x, y) on the top surface (Fig. 3.4). Equation (3.6) is known as the paraxial approximation of the gaussian beam.
3.3. Powder properties
In the case we studyλ = 1070 nm, ω = 40 µm (see Tab. 3.4), and the condition (3.5) for the paraxial approximation is: z ¿ 9.3 mm. Therefore for powder layers up to several hundreds microns thick the propagation of the gaussian beam can be described by (3.6).
The optical penetration depth is a measure of light propagation in the material. It is defined as the depth at which the radiation intensity inside the material falls to 1/e of its original value at the surface. Generally, for bulk metals, the optical penetration depth is of the order of tens of nanometers . As we can see from (3.4), if the optical penetration depth is small compare to the thickness of the materialδ ¿ ∆z, we can neglect the transmitted part of the radiation Itr. The incident radiation falling onto a powder bed is not only partially absorbed by the outer surface but also penetrates through the pores due to multiple reflections. For metallic powders with grain size of 10 − 20 µm, δ is of the order of several powder particle diameters . Therefore in laser sintering/melting of a powder layer with a thickness less than hundred microns, the penetration depth plays an important role in laser energy deposition. The influence ofδ increases for highly reflective metallic powders .
Estimation of the parameters of laser energy deposition onto a powder bed was an objective of many studies [7, 17, 41, 43, 55, 56]. The principal question, arising with regard to the radiation transfer during laser treatment of powders, is the influence of the wavelength, material, particle size, packing structure and density. The subject was studied experimentally , by ray-tracing modeling [7, 43] and by solving the radiation transfer equation (RTE) .
Several techniques for measuring powder absorptivity/reflectivity currently exist [56, 57, 58]. One of the most reliable methods was applied by N.K. Tolochko (so-called radiometric tech-nique). He used an integrating sphere for direct measurement of a powder absorptivity. The radiometric technique was applied in LGPP for 18Ni(300) Maraging Steel powder . Experiments showed that the effective absorptivity of the powder is quite high compare to the absorptivity of the bulk material:αexpp = 0.7 − 0.8.
These experimental results are confirmed by the solution of the radiation transfer equation (RTE), which was performed by A.V. Gusarov in . In his method he applies the statistical scattering model to a powder bed. In the model radiative properties in packed powder beds of non-spherical particles with arbitrary orientation (statistically isotropic powder bed) are expressed as the properties of packed beds of spherical particles with the same porosity and specific surface.
According to the Gusarov’s solution of RTE the effective absorptivity of 18Ni(300) Maraging Steel powder bed is in the rangeαtheorp = 0.78 − 0.88. This theoretical estimation is in good correspondence with the results obtained by means of the integrating sphereαexpp . In our simulation we will use the valueαp= 0.8 for the effective absorptivity of 18Ni(300) Maraging Steel powder.
Chapter 3. 18Ni(300) Maraging Steel Powder
Figure 3.5 – Discrete thermal resistances model for powder beds by A.V. Gusarov (pic. ).
Experiments for the definition of the optical penetration depth were also performed by means of the integrating sphere [59, 60]. According to the results, the penetration depth of 18Ni(300) Maraging Steel loose powder isδ ' 20 µm.
3.3.2 Powder density
The value of 18Ni(300) Maraging Steel powder densityρpcan vary from 50% to 70% of the densityρsof the solid material. In most of our simulations we will consider the case of a very loose powder: we assume that the powder densityρpis 50% of the density of the bulk material ρp= 0.5ρs= 0.004 g/mm3(see Tab. 3.2).
3.3.3 Effective thermal conductivity
In the framework of the homogeneous medium hypothesis we usually use the concept of effective thermal conductivity for powders. The effective thermal conductivity relates to a certain volume (greater than the size of inhomogeneity) of the material and describes the heat conduction of this volume as a whole. A powder bed is considered as a multiphase heterogeneous medium, where the solid particles are dispersed in a continuous gas phase in such a way that they can touch each other and form point contacts between them. Therefore, the effective thermal conductivity of a powder depends both on the properties of the solid and of the gas phases.
The model of effective thermal conductivity developed by A.V. Gusarov  takes into account all the types of thermal interaction between particles in powder and packed beds. This model, applied to packed equal spheres, estimates the effective thermal conductivity as a function of the volume fraction of solid fs, the mean coordination number N , and the thermal resistance of a contact between two neighbouring particlesΣp.
3.3. Powder properties
Powder type d0 fs kp(eq.(3.7)) kp(exp.)
18Ni(300) Maraging Steel 8.87µm 50 − 55% 0.0982 W/m/◦C 0.0847 W/m/◦C
Commercially Pure Silver 5µm 60% 0.0857 W/m/◦C 0.0949 W/m/◦C
Table 3.3 – Thermal conductivity of powders in air at normal conditions: theoretical prediction and experimental results.
The contact resistanceΣpdepends on four dimensionless parameters: the relative size of the contact rc/r0between powder grains, the ratio of thermal conductivities of the solid and gas phases ks/kg, the Knudsen number Kn, and the adiabatic exponent of the gas phaseγa. If the particles of an heterogeneous medium form only point contacts (as in the case of loose powders), the heat flux through the solid phase is negligible and the heat transfer is performed through the gas gap between powder particles.
For point contacts rc' 0, at high ks/kg, as it is in a powder bed:
kp kg = fsN 2 · 1 2ln(1 + L) + ln(1 + p L) + 1 1 +pL− 1 ¸ L =4pπKn3 γa+ 1 9γa− 5 , Kn = l0/d0, (3.7)
where l0is a gas mean-free path, d0- powder grain diameter.
In this study k is the notation of the effective thermal conductivity of the material. In order to denote the effective thermal conductivities of the powder and of the solid material we use kp and ks, respectively.
For the validation of the theory, described above, an experimental setup for powder conduc-tivity measurements, based on the classical flash method , was developed . The first experimental results for several powder types are presented in Tab. 3.3. They are compared to theoretical prediction of Gusarov’s theory for point contacts (3.7).
In the theoretical estimation of the effective thermal conductivity of powders we assume that air plays the role of the gas phase between powder particles: γa= 7/5, kg= 0.026 W/m/◦C, l0= 58 nm . The coordination number N = 5.57 corresponds to a randomly packed powder bed (see ).
The results in Tab. 3.3 show that the effective thermal conductivity of a powder is of the order of several times the conductivity of air and depends on the particles diameter. One can see good correlation between theory and practice for maraging steel and pure silver powders. In the simulation we will use the value kp= 0.1 W/m/◦C for the effective thermal conductivity of 18Ni(300) Maraging Steel powder.
Chapter 3. 18Ni(300) Maraging Steel Powder
3.4 Molten material properties
In this study we assume that the thermal conductivity kl of the liquid 18Ni(300) Maraging Steel is similar to the value ksfor the solid material and is not dependent on temperature. According to , the thermal expansion coefficient for different grades of steels at the melting point does not exceed 2 · 10−51/◦C. Therefore the densityρl of molten 18Ni(300) Maraging Steel is approximately equal to the densityρs of the solid material. However the same assumption cannot be made for the material surface absorptivity, which evolves significantly during melting.
According to [56, 64, 65] absorptivity of a flat solid stainless steel surface for a wavelength close to 1µm at the room temperature is in the range 0.4 − 0.6, depending on the roughness of the surface. Whereas the surface absorptivity of liquid steel can vary from 0.1 to 0.3 for the same wavelength [64, 65].
In this work we choose the valuesαl= 0.2 and αs= 0.5 for the surface absorptivity of molten and solid 18Ni(300) Maraging Steel, respectively.
Remark 3.1. Actually the surface absorptivity of molten steel strongly depends on its chemical
composition and on the interaction with the surrounding atmosphere. For example, oxidation of the liquid material surface can cause a significant increase of absorptivity: up to 0.7, according to [64, 66]. However in this study we assume that the surface oxidation is negligible. This assumption is justified since the SLS/SLM process is performed under a protective atmosphere (argon Ar).
3.5. Operation parameters used for Maraging Steel Powder
Laser wavelengthλ 1070 nm
Laser beam profile top-hat/gaussian Laser beam radiusω 40 µm
Laser power P 100; 200; 300 W
Scanning speedυ 1; 2; 3 m/s
Table 3.4 – Process parameters used in the study.
3.5 Operation parameters used for Maraging Steel Powder
The typical process parameters, used in this study, are presented in Tab. 3.4. We have chosen them in accordance with modern industrial requirements (see Chapter 2). The parameters form 9 sets (see Tab. 3.5). However some of them will not give good results for the chosen laser and material parameters. We will discuss it in next chapters.
The choice of the scanning strategy and of the dimensions of the powder layer will be discussed in each chapter separately.
Set No. Power/speed, W/(m/s)
1 100/1 2 100/2 3 100/3 4 200/1 5 200/2 6 200/3 7 300/1 8 300/2 9 300/3
Chapter 3. 18Ni(300) Maraging Steel Powder
Parameter Powder bed Solid material Liquid material
Grain radius r0 4.435µm − −
Optical penetration depthδ 20 µm − −
Absorptivityα 0.8 0.5 0.2
Thermal conductivity k 0.1 W/m/◦C 26 W/m/◦C 26 W/m/◦C
Densityρ 0.004 g/mm3 0.008 g/mm3 0.008 g/mm3
Table 3.6 – Properties of 18Ni(300) Maraging Steel.
Tab. 3.6 summarizes the properties of 18Ni(300) Maraging Steel powder, solid and liquid material, which we will use in the study.
It can be seen that, during sintering/melting of 18Ni(300) Maraging Steel, the thermal con-ductivity and the absorptivity of the material change drastically. Thermal concon-ductivity of the powder is of the order of several times the conductivity of air but it is less than 1% of the conductivity of bulk material. At the same time the liquid material (as all liquid metals) is highly reflective, while the powder bed effectively absorbs laser energy. In the next chapters, we will discuss the influence of these phenomena on the SLS/SLM process.
Observe that such a significant change in the properties due to melting is typical for the majority of metallic powders used in SLS/SLM.
Single Grain Model
In this Chapter we consider the mechanisms of heating and melting of a separate and perfectly spherical powder grain irradiated by a plane electromagnetic wave. This theory is often called Single Grain Model (SGM) [38, 67]. We improve the existing model by considering the real intensity distribution instead of the homogeneous one and by taking the finite thermal conductivity of a powder particle into account.
The main outputs of the Single Grain Model will be:
• an estimation of the melting time of a grain;
• a relatively precise information about the evolution of the average temperature inside a grain.
These results will be used later on to build the reliable consolidation model we need to integrate into the macroscopic description of the SLS/SLM process.
Chapter 4. Single Grain Model
Figure 4.1 – Irradiation of the surface of a powder bed by a moving laser.
4.1 Single Grain Model: main assumptions
Evolution of the effective parameters of a powder bed depends on the melting dynamics of powder grains and their interaction and rearrangement. A Single Grain Model allows to study the process of melting of a separate powder grain on the surface of a powder bed during laser heating. Knowing the melting behavior of a single grain we can better understand the evolution mechanisms of powder properties during laser sintering/melting.
The Single Grain Model considers powder-laser interaction at a scale of a powder grain size. The grain is assumed to be spherical and there is no influence of the neighbouring grains. Remark 4.1. In [38, 67] the grain was assumed to be homogeneously irradiated all over its
surface. Since homogeneous irradiation is difficult to justify, in this study we consider that the powder particle interacts with a monochromatic polarized plane wave (see Fig. 4.1), which is a rough approximation of a top-hat/gaussian laser beam. However we will keep the name ‘Single Grain Model’ for this theory.
In a plane electromagnetic wave, linearly polarized in the direction of x-axis and propagating in the void along z-axis (see Fig. 4.1), the electric field at a moment of time t = 0 in a point (x, y, z) is:
E(x, y, z, t ) = E0e−i (kλz−ωft )= E0e−i (kλz−ωft )ex. (4.1)
The wave is characterized by its electric amplitude E0, the wave number kλ= 2π/λ and the angular frequencyωf = kλc with c the speed of the light.
4.1. Single Grain Model: main assumptions
Laser wavelengthλ 1070 nm
Laser beam radiusω 40µm
Laser beam profile top-hat/gaussian
Radius of the grain r0 4.435µm
Densityρs 0.008 g/mm3
Thermal conductivity ks 0.026 W/mm/◦C Dielectric constantεR+i εI (3.24 − i 4.34)2 Latent heat of fusion Lf 247 J/g
Table 4.1 – Properties of the laser and of a typical 18Ni(300) Maraging Steel powder grain.
4.1.1 Intensity of the plane wave and laser power
An important characteristic of an electromagnetic plane wave is its time-average intensity I0. This field proves to be constant in space and oriented in the direction of the wave propagation:
I0(x, y, z) = I0ez. (4.2)
For the plane wave (4.1), the connection between I0and the electric amplitude is: I0=
whereµp= 4π · 10−7N/A2is the vacuum magnetic permeability.
In the Single Grain Model the plane wave we select to approach the laser beam, has a time-average intensity I0equal to the maximum laser beam intensity:
for the top-hat or gaussian beam. We use the expression (4.4) both for the top-hat and gaussian beam, as far as we assume that powder particles we are interested in, i.e. the particles which are molten, are situated in the center of the laser beam.
Chapter 4. Single Grain Model
z (polar axis)
e.-m. wave polarisation
Figure 4.2 – Meshing of a 2D domain for the Single Grain Model calculations.
4.1.2 Heating of a spherical grain with a plane wave
The heating by a plane electromagnetic wave of amplitude E0of a non-magnetic spherical particle with a complex dielectric constantεd= εR+ i εI, can be described by Mie theory . It allows to express the electric field, transmitted to the sphere, in the form:
E = kE0ke, (4.5)
where e is the field transmitted for an incident wave with unit electric amplitude.
Using Mie solution of Maxwell equations, we can calculate the heat source q induced by Joule heating in the irradiated powder grain. It is proportional to the intensity I0:
q =1 δI0∥ e ∥ 2. (4.6) The factor δ = − 1 εIkλ (4.7)
in (4.6) has the dimension of a length and corresponds to the optical penetration depth of the grain.
As we discussed in § 3.3.1 of Chapter 3, penetration depths of bulk metals are relatively small (tens of nanometers) compare to the radius of the grain (r0= 4.435 µm). Therefore the volume source (4.6) is concentrated near its surface and a finite element simulation of the heating process would require a very fine meshing of the grain. The classical solution to avoid this issue is to replace the volume heat source (4.6) by an equivalent surface heat source qsurf:
qsurf= −I0n · st. (4.8)
4.2. Melting of a powder grain
Figure 4.3 – Temperature distribution inside a spherical grain after 6µs of irradiation by the plane wave with the intensity corresponding to the 100 W laser (Tab. 4.1).
In (4.8) stdenotes the Poynting vector, transmitted to the sphere in the case of an incident
plane wave with unit intensity.
In the case of a linearly polarized wave, the heat source has a simple dependency with respect to the polar angleϕ (Fig. 4.2). If the polar axis is aligned with the direction of wave propagation (z-axis in our case), we can write that:
qsurf(r, z,ϕ) = I0(b0(r, z) + b1(r, z) cos 2ϕ), (4.9)
where (r, z,ϕ) are the cylindrical coordinates and where b0and b1are functions of r and z only. The coefficients b0and b1can be calculated numerically by means of a simulation tool .
4.2 Melting of a powder grain
Using the theory presented above, we can model numerically the melting process of a separate spherical powder grain of radius r0irradiated by a laser beam of intensity I0. The properties of the grain correspond to a typical particle in a 18Ni(300) Maraging Steel powder bed. They are listed in Tab. 4.1. The dielectric constantεdcorresponds to the value for steel .
The mesh used to discretize the grain surface is presented in Fig. 4.2 in polar symmetry. In this context we can study the evolution of the temperature field in the particle and its melting during irradiation with a standard finite element method.